#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/62/4306276.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4306276
loop_
_publ_author_name
'Ghada A. Al-Kadamany'
'Firasat Hussain'
'Sib Sankar Mal'
'Michael H. Dickman'
'Nathalie Leclerc-Laronze'
'Jérôme Marrot'
'Emmanuel Cadot'
'Ulrich Kortz'
_publ_section_title
;
Cyclic Ti9 Keggin Trimers with Tetrahedral (PO4) or Octahedral (TiO6)
Capping Groups
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              8574
_journal_page_last               8576
_journal_paper_doi               10.1021/ic801114n
_journal_volume                  47
_journal_year                    2008
_chemical_formula_sum            'Cs11.5 K1.5 Na1.5 O134 Si3 Ti10 W27'
_chemical_formula_weight         9292.82
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           160
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   30.3253(11)
_cell_length_b                   30.3253(11)
_cell_length_c                   15.8808(14)
_cell_measurement_reflns_used    8835
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.90
_cell_measurement_theta_min      2.42
_cell_volume                     12647.7(13)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0426
_diffrn_reflns_av_sigmaI/netI    0.0276
_diffrn_reflns_limit_h_max       42
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       37
_diffrn_reflns_limit_k_min       -42
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            89174
_diffrn_reflns_theta_full        30.05
_diffrn_reflns_theta_max         30.05
_diffrn_reflns_theta_min         1.34
_exptl_absorpt_coefficient_mu    21.374
_exptl_absorpt_correction_T_max  0.4819
_exptl_absorpt_correction_T_min  0.1836
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.660
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       parallelepiped
_exptl_crystal_F_000             12029
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.243
_refine_diff_density_min         -2.119
_refine_diff_density_rms         0.763
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.003(8)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.233
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     346
_refine_ls_number_reflns         8660
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.232
_refine_ls_R_factor_all          0.0389
_refine_ls_R_factor_gt           0.0258
_refine_ls_shift/su_max          0.009
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0564P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0720
_refine_ls_wR_factor_ref         0.0937
_reflns_number_gt                7788
_reflns_number_total             8660
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic801114n_si_001_2.cif
_cod_data_source_block           natl54sa
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Trigonal' changed to 'trigonal' according
to '/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum        'Cs11.50 K1.50 Na1.50 O134 Si3 Ti10 W27'
_cod_database_code               4306276
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.499992(4) 0.999985(7) 0.361264(17) 0.02875(5) Uani 1 2 d S . .
W2 W 0.446102(5) 1.003075(5) 0.544918(12) 0.02980(4) Uani 1 1 d . . .
W3 W 0.499779(5) 0.888822(5) 0.684134(10) 0.02615(3) Uani 1 1 d . . .
W4 W 0.560874(4) 0.887013(5) 0.480763(11) 0.02551(3) Uani 1 1 d . . .
W5 W 0.503290(5) 0.883389(5) 0.298028(10) 0.02602(3) Uani 1 1 d . . .
Ti1 Ti 0.454570(19) 0.785534(19) 0.42986(4) 0.02009(14) Uani 1 1 d . . .
Ti2 Ti 0.394059(14) 0.78812(3) 0.61871(6) 0.01817(17) Uani 1 2 d S . .
Ti3 Ti 0.3333 0.6667 0.72663(10) 0.0229(3) Uani 1 6 d S . .
Si1 Si 0.44469(2) 0.88938(4) 0.48721(8) 0.0163(2) Uani 1 2 d S . .
O1 O 0.52221(7) 1.04443(15) 0.2817(3) 0.0399(11) Uani 1 2 d S . .
O2 O 0.43440(9) 0.95393(8) 0.32506(19) 0.0305(7) Uani 1 1 d . . .
O3 O 0.55889(9) 1.03086(9) 0.4344(2) 0.0330(8) Uani 1 1 d . . .
O4 O 0.47581(6) 0.95162(12) 0.4854(2) 0.0219(8) Uani 1 2 d S . .
O5 O 0.43331(11) 1.04879(9) 0.5849(3) 0.0460(10) Uani 1 1 d . . .
O6 O 0.42709(9) 0.95743(9) 0.6356(2) 0.0361(8) Uani 1 1 d . . .
O7 O 0.38417(9) 0.95652(9) 0.4953(2) 0.0305(7) Uani 1 1 d . . .
O8 O 0.51662(6) 1.03324(13) 0.5790(3) 0.0316(10) Uani 1 2 d S . .
O9 O 0.54110(10) 0.90095(11) 0.7669(2) 0.0371(8) Uani 1 1 d . . .
O10 O 0.45551(8) 0.82020(8) 0.69516(17) 0.0254(6) Uani 1 1 d . . .
O11 O 0.53520(8) 0.87794(8) 0.59368(18) 0.0281(7) Uani 1 1 d . . .
O12 O 0.45209(7) 0.90417(15) 0.7402(2) 0.0291(9) Uani 1 2 d S . .
O13 O 0.43511(6) 0.87022(12) 0.5844(2) 0.0227(8) Uani 1 2 d S . .
O14 O 0.62236(8) 0.89941(9) 0.4963(2) 0.0351(8) Uani 1 1 d . . .
O15 O 0.52688(8) 0.81791(8) 0.46203(17) 0.0257(6) Uani 1 1 d . . .
O16 O 0.56472(9) 0.89945(9) 0.3607(2) 0.0315(7) Uani 1 1 d . . .
O17 O 0.47815(8) 0.86860(8) 0.43916(17) 0.0238(6) Uani 1 1 d . . .
O18 O 0.52765(10) 0.89369(10) 0.1976(2) 0.0388(8) Uani 1 1 d . . .
O19 O 0.47878(9) 0.81459(8) 0.31391(17) 0.0278(7) Uani 1 1 d . . .
O20 O 0.43639(6) 0.87278(13) 0.2776(3) 0.0290(9) Uani 1 2 d S . .
O21 O 0.44576(14) 0.72288(7) 0.4067(2) 0.0238(8) Uani 1 2 d S . .
O22 O 0.43171(8) 0.77640(8) 0.53754(16) 0.0237(6) Uani 1 1 d . . .
O23 O 0.38645(7) 0.77289(14) 0.3889(2) 0.0260(8) Uani 1 2 d S . .
O24 O 0.36325(6) 0.72649(13) 0.6714(3) 0.0282(9) Uani 1 2 d S . .
O25 O 0.30204(15) 0.69796(15) 0.8150(4) 0.096(2) Uani 1 2 d S . .
Cs1 Cs 0.3333 0.6667 0.48793(4) 0.02471(12) Uani 1 6 d S . .
Cs2 Cs 0.579815(8) 1.159631(15) 0.30578(3) 0.04335(10) Uani 1 2 d S . .
Cs3 Cs 0.645148(12) 1.015610(11) 0.33758(3) 0.05696(10) Uani 1 1 d . . .
Cs4 Cs 0.48942(3) 0.97884(7) 0.11956(10) 0.0917(5) Uani 0.50 2 d SP . .
K1 K 0.5811(2) 0.79055(10) 0.3207(3) 0.1101(14) Uani 0.50 2 d SP . .
Na1 Na 0.4094(5) 1.1121(5) 0.5911(12) 0.058(3) Uani 0.13 1 d P . .
Na2 Na 0.5122(5) 0.8657(6) -0.0038(12) 0.058(3) Uani 0.13 1 d P . .
O1W O 0.4801(6) 0.7401(3) 0.2005(7) 0.105(4) Uani 0.67 2 d SP . .
O2W O 0.3661(3) 0.7322(7) 0.2300(9) 0.102(4) Uani 0.50 2 d SP . .
O3W O 0.3763(6) 1.0818(5) 0.7223(10) 0.069(5) Uani 0.25 1 d P . .
O4W O 0.3989(4) 0.7979(9) 0.8703(15) 0.131(7) Uiso 0.50 2 d SP . .
O5W O 0.4567(6) 0.9134(12) 1.027(2) 0.192(12) Uiso 0.50 2 d SP . .
O6W O 0.3407(8) 0.6814(17) -0.001(2) 0.151(15) Uiso 0.25 2 d SP . .
O7W O 0.5120(5) 1.0241(10) 0.7821(18) 0.160(10) Uiso 0.50 2 d SP . .
O8W O 0.4256(5) 0.8513(10) 0.0559(18) 0.160(10) Uiso 0.50 2 d SP . .
O9W O 0.4598(6) 0.9196(11) 0.9400(17) 0.173(11) Uiso 0.50 2 d SP . .
O10W O 0.4763(11) 0.953(2) 0.895(3) 0.153(18) Uiso 0.25 2 d SP . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 W1 O2 102.38(14) . 5 ?
O1 W1 O2 102.38(14) . . ?
O2 W1 O2 87.90(19) 5 . ?
O1 W1 O3 99.00(14) . . ?
O2 W1 O3 89.16(14) 5 . ?
O2 W1 O3 158.56(12) . . ?
O1 W1 O3 99.00(14) . 5 ?
O2 W1 O3 158.56(12) 5 5 ?
O2 W1 O3 89.16(14) . 5 ?
O3 W1 O3 85.9(2) . 5 ?
O1 W1 O4 170.05(17) . . ?
O2 W1 O4 84.70(11) 5 . ?
O2 W1 O4 84.70(11) . . ?
O3 W1 O4 73.88(10) . . ?
O3 W1 O4 73.88(10) 5 . ?
O1 W1 Cs4 50.98(15) . . ?
O2 W1 Cs4 66.48(9) 5 . ?
O2 W1 Cs4 66.48(9) . . ?
O3 W1 Cs4 130.85(9) . . ?
O3 W1 Cs4 130.86(9) 5 . ?
O4 W1 Cs4 138.97(9) . . ?
O1 W1 Cs3 82.414(7) . 5 ?
O2 W1 Cs3 136.37(9) 5 5 ?
O2 W1 Cs3 49.30(9) . 5 ?
O3 W1 Cs3 133.47(10) . 5 ?
O3 W1 Cs3 48.52(10) 5 5 ?
O4 W1 Cs3 97.361(7) . 5 ?
Cs4 W1 Cs3 85.723(7) . 5 ?
O1 W1 Cs3 82.414(7) . . ?
O2 W1 Cs3 49.30(9) 5 . ?
O2 W1 Cs3 136.36(9) . . ?
O3 W1 Cs3 48.52(10) . . ?
O3 W1 Cs3 133.47(10) 5 . ?
O4 W1 Cs3 97.361(7) . . ?
Cs4 W1 Cs3 85.722(7) . . ?
Cs3 W1 Cs3 164.776(12) 5 . ?
O1 W1 Cs2 35.39(15) . . ?
O2 W1 Cs2 124.94(9) 5 . ?
O2 W1 Cs2 124.94(9) . . ?
O3 W1 Cs2 73.34(8) . . ?
O3 W1 Cs2 73.34(8) 5 . ?
O4 W1 Cs2 134.67(8) . . ?
Cs4 W1 Cs2 86.37(3) . . ?
Cs3 W1 Cs2 83.455(5) 5 . ?
Cs3 W1 Cs2 83.455(5) . . ?
O5 W2 O7 102.48(14) . . ?
O5 W2 O6 101.51(16) . . ?
O7 W2 O6 86.79(12) . . ?
O5 W2 O3 100.82(14) . 5 ?
O7 W2 O3 88.98(13) . 5 ?
O6 W2 O3 157.66(12) . 5 ?
O5 W2 O8 98.96(14) . . ?
O7 W2 O8 158.55(13) . . ?
O6 W2 O8 89.64(15) . . ?
O3 W2 O8 86.33(16) 5 . ?
O5 W2 O4 171.22(11) . . ?
O7 W2 O4 84.44(11) . . ?
O6 W2 O4 84.12(13) . . ?
O3 W2 O4 73.64(11) 5 . ?
O8 W2 O4 74.16(11) . . ?
O5 W2 Cs3 58.55(9) . 12_465 ?
O7 W2 Cs3 60.77(10) . 12_465 ?
O6 W2 Cs3 61.15(9) . 12_465 ?
O3 W2 Cs3 133.80(9) 5 12_465 ?
O8 W2 Cs3 134.15(12) . 12_465 ?
O4 W2 Cs3 130.19(7) . 12_465 ?
O5 W2 Cs3 82.07(13) . 5 ?
O7 W2 Cs3 48.68(9) . 5 ?
O6 W2 Cs3 134.28(8) . 5 ?
O3 W2 Cs3 50.28(10) 5 5 ?
O8 W2 Cs3 135.33(13) . 5 ?
O4 W2 Cs3 98.90(8) . 5 ?
Cs3 W2 Cs3 84.420(8) 12_465 5 ?
O9 W3 O10 102.17(13) . . ?
O9 W3 O11 101.40(14) . . ?
O10 W3 O11 91.80(11) . . ?
O9 W3 O12 98.53(15) . . ?
O10 W3 O12 91.02(14) . . ?
O11 W3 O12 158.80(13) . . ?
O9 W3 O6 99.54(14) . 5 ?
O10 W3 O6 158.28(13) . 5 ?
O11 W3 O6 83.10(12) . 5 ?
O12 W3 O6 86.55(15) . 5 ?
O9 W3 O13 172.50(12) . . ?
O10 W3 O13 75.15(12) . . ?
O11 W3 O13 85.77(10) . . ?
O12 W3 O13 74.67(12) . . ?
O6 W3 O13 83.41(13) 5 . ?
O9 W3 Ti2 134.72(9) . . ?
O10 W3 Ti2 32.82(9) . . ?
O11 W3 Ti2 88.48(6) . . ?
O12 W3 Ti2 82.59(11) . . ?
O6 W3 Ti2 125.62(10) 5 . ?
O13 W3 Ti2 42.33(8) . . ?
O9 W3 Cs3 53.82(9) . 8_665 ?
O10 W3 Cs3 128.91(9) . 8_665 ?
O11 W3 Cs3 58.05(6) . 8_665 ?
O12 W3 Cs3 132.48(11) . 8_665 ?
O6 W3 Cs3 65.23(9) 5 8_665 ?
O13 W3 Cs3 133.28(8) . 8_665 ?
Ti2 W3 Cs3 144.893(12) . 8_665 ?
O9 W3 Cs2 87.22(11) . 8_665 ?
O10 W3 Cs2 44.58(9) . 8_665 ?
O11 W3 Cs2 53.71(8) . 8_665 ?
O12 W3 Cs2 135.06(12) . 8_665 ?
O6 W3 Cs2 136.67(9) 5 8_665 ?
O13 W3 Cs2 95.38(7) . 8_665 ?
Ti2 W3 Cs2 63.378(9) . 8_665 ?
Cs3 W3 Cs2 86.261(8) 8_665 8_665 ?
O14 W4 O15 101.56(12) . . ?
O14 W4 O11 102.38(14) . . ?
O15 W4 O11 91.82(11) . . ?
O14 W4 O16 98.34(14) . . ?
O15 W4 O16 90.43(11) . . ?
O11 W4 O16 158.25(12) . . ?
O14 W4 O7 99.00(12) . 5 ?
O15 W4 O7 159.44(12) . 5 ?
O11 W4 O7 83.44(12) . 5 ?
O16 W4 O7 86.90(13) . 5 ?
O14 W4 O17 171.97(13) . . ?
O15 W4 O17 76.27(10) . . ?
O11 W4 O17 85.47(10) . . ?
O16 W4 O17 74.07(10) . . ?
O7 W4 O17 83.40(11) 5 . ?
O14 W4 Ti1 133.86(9) . . ?
O15 W4 Ti1 32.51(8) . . ?
O11 W4 Ti1 87.56(6) . . ?
O16 W4 Ti1 82.78(6) . . ?
O7 W4 Ti1 127.02(9) 5 . ?
O17 W4 Ti1 43.80(6) . . ?
O14 W4 Cs3 53.54(11) . 8_665 ?
O15 W4 Cs3 128.15(9) . 8_665 ?
O11 W4 Cs3 58.82(6) . 8_665 ?
O16 W4 Cs3 133.07(6) . 8_665 ?
O7 W4 Cs3 65.59(9) 5 8_665 ?
O17 W4 Cs3 133.79(7) . 8_665 ?
Ti1 W4 Cs3 144.151(13) . 8_665 ?
O14 W4 Cs3 77.36(10) . . ?
O15 W4 Cs3 135.97(9) . . ?
O11 W4 Cs3 131.85(7) . . ?
O16 W4 Cs3 47.38(7) . . ?
O7 W4 Cs3 50.02(9) 5 . ?
O17 W4 Cs3 98.72(6) . . ?
Ti1 W4 Cs3 127.644(13) . . ?
Cs3 W4 Cs3 87.103(8) 8_665 . ?
O14 W4 Cs2 88.97(10) . 8_665 ?
O15 W4 Cs2 45.13(9) . 8_665 ?
O11 W4 Cs2 52.22(8) . 8_665 ?
O16 W4 Cs2 135.37(8) . 8_665 ?
O7 W4 Cs2 135.55(9) 5 8_665 ?
O17 W4 Cs2 94.67(6) . 8_665 ?
Ti1 W4 Cs2 61.860(13) . 8_665 ?
Cs3 W4 Cs2 85.878(10) 8_665 8_665 ?
Cs3 W4 Cs2 166.249(8) . 8_665 ?
O18 W5 O19 103.02(13) . . ?
O18 W5 O20 101.31(17) . . ?
O19 W5 O20 92.24(13) . . ?
O18 W5 O16 99.12(14) . . ?
O19 W5 O16 90.40(11) . . ?
O20 W5 O16 158.23(15) . . ?
O18 W5 O2 98.75(13) . 5 ?
O19 W5 O2 158.23(12) . 5 ?
O20 W5 O2 83.63(13) . 5 ?
O16 W5 O2 85.93(12) . 5 ?
O18 W5 O17 173.50(13) . . ?
O19 W5 O17 75.18(10) . . ?
O20 W5 O17 85.05(14) . . ?
O16 W5 O17 74.75(11) . . ?
O2 W5 O17 83.16(10) 5 . ?
O18 W5 Ti1 135.01(11) . . ?
O19 W5 Ti1 32.42(9) . . ?
O20 W5 Ti1 89.77(11) . . ?
O16 W5 Ti1 80.98(8) . . ?
O2 W5 Ti1 125.93(9) 5 . ?
O17 W5 Ti1 42.78(6) . . ?
O18 W5 Cs3 79.85(8) . . ?
O19 W5 Cs3 134.19(8) . . ?
O20 W5 Cs3 132.61(10) . . ?
O16 W5 Cs3 44.88(8) . . ?
O2 W5 Cs3 50.01(9) 5 . ?
O17 W5 Cs3 96.87(5) . . ?
Ti1 W5 Cs3 122.965(12) . . ?
O18 W5 Cs4 55.49(12) . . ?
O19 W5 Cs4 138.07(9) . . ?
O20 W5 Cs4 62.69(11) . . ?
O16 W5 Cs4 125.66(8) . . ?
O2 W5 Cs4 57.51(9) 5 . ?
O17 W5 Cs4 129.86(7) . . ?
Ti1 W5 Cs4 152.330(17) . . ?
Cs3 W5 Cs4 81.48(2) . . ?
O22 Ti1 O21 100.72(14) . . ?
O22 Ti1 O15 94.41(11) . . ?
O21 Ti1 O15 96.81(14) . . ?
O22 Ti1 O23 89.89(14) . . ?
O21 Ti1 O23 97.76(15) . . ?
O15 Ti1 O23 163.77(13) . . ?
O22 Ti1 O19 163.02(12) . . ?
O21 Ti1 O19 95.90(14) . . ?
O15 Ti1 O19 87.00(11) . . ?
O23 Ti1 O19 84.42(13) . . ?
O22 Ti1 O17 89.56(10) . . ?
O21 Ti1 O17 168.42(14) . . ?
O15 Ti1 O17 76.93(10) . . ?
O23 Ti1 O17 87.47(12) . . ?
O19 Ti1 O17 74.25(10) . . ?
O22 Ti1 W4 91.86(6) . . ?
O21 Ti1 W4 126.62(12) . . ?
O15 Ti1 W4 30.11(8) . . ?
O23 Ti1 W4 134.25(10) . . ?
O19 Ti1 W4 80.88(6) . . ?
O17 Ti1 W4 46.85(6) . . ?
O22 Ti1 W5 134.23(8) . . ?
O21 Ti1 W5 125.03(12) . . ?
O15 Ti1 W5 80.26(8) . . ?
O23 Ti1 W5 85.53(11) . . ?
O19 Ti1 W5 29.47(7) . . ?
O17 Ti1 W5 44.79(7) . . ?
W4 Ti1 W5 61.515(10) . . ?
O22 Ti1 Cs1 60.39(6) . . ?
O21 Ti1 Cs1 59.02(11) . . ?
O15 Ti1 Cs1 136.56(8) . . ?
O23 Ti1 Cs1 58.48(11) . . ?
O19 Ti1 Cs1 127.73(6) . . ?
O17 Ti1 Cs1 131.91(7) . . ?
W4 Ti1 Cs1 151.38(2) . . ?
W5 Ti1 Cs1 142.99(2) . . ?
O22 Ti1 Cs2 49.38(9) . 8_665 ?
O21 Ti1 Cs2 77.51(12) . 8_665 ?
O15 Ti1 Cs2 55.10(8) . 8_665 ?
O23 Ti1 Cs2 135.75(11) . 8_665 ?
O19 Ti1 Cs2 139.62(8) . 8_665 ?
O17 Ti1 Cs2 105.90(7) . 8_665 ?
W4 Ti1 Cs2 72.400(13) . 8_665 ?
W5 Ti1 Cs2 133.420(15) . 8_665 ?
Cs1 Ti1 Cs2 83.141(15) . 8_665 ?
O22 Ti1 K1 132.55(11) . . ?
O21 Ti1 K1 66.63(12) . . ?
O15 Ti1 K1 46.41(11) . . ?
O23 Ti1 K1 135.71(13) . . ?
O19 Ti1 K1 58.22(10) . . ?
O17 Ti1 K1 102.47(7) . . ?
W4 Ti1 K1 66.92(6) . . ?
W5 Ti1 K1 73.31(4) . . ?
Cs1 Ti1 K1 125.60(4) . . ?
Cs2 Ti1 K1 83.30(7) 8_665 . ?
O24 Ti2 O22 99.79(12) . . ?
O24 Ti2 O22 99.80(12) . 5 ?
O22 Ti2 O22 89.75(16) . 5 ?
O24 Ti2 O10 95.43(12) . 5 ?
O22 Ti2 O10 164.57(11) . 5 ?
O22 Ti2 O10 90.11(11) 5 5 ?
O24 Ti2 O10 95.43(12) . . ?
O22 Ti2 O10 90.11(11) . . ?
O22 Ti2 O10 164.57(11) 5 . ?
O10 Ti2 O10 85.96(17) 5 . ?
O24 Ti2 O13 166.86(16) . . ?
O22 Ti2 O13 89.47(10) . . ?
O22 Ti2 O13 89.47(10) 5 . ?
O10 Ti2 O13 75.10(10) 5 . ?
O10 Ti2 O13 75.10(10) . . ?
O24 Ti2 W3 124.57(10) . . ?
O22 Ti2 W3 89.43(6) . . ?
O22 Ti2 W3 135.05(7) 5 . ?
O10 Ti2 W3 79.83(8) 5 . ?
O10 Ti2 W3 29.51(7) . . ?
O13 Ti2 W3 45.59(7) . . ?
O24 Ti2 W3 124.57(10) . 5 ?
O22 Ti2 W3 135.06(7) . 5 ?
O22 Ti2 W3 89.42(6) 5 5 ?
O10 Ti2 W3 29.51(7) 5 5 ?
O10 Ti2 W3 79.83(8) . 5 ?
O13 Ti2 W3 45.59(7) . 5 ?
W3 Ti2 W3 61.158(15) . 5 ?
O24 Ti2 Cs1 60.39(13) . . ?
O22 Ti2 Cs1 59.06(6) . . ?
O22 Ti2 Cs1 59.07(6) 5 . ?
O10 Ti2 Cs1 132.65(8) 5 . ?
O10 Ti2 Cs1 132.65(8) . . ?
O13 Ti2 Cs1 132.75(10) . . ?
W3 Ti2 Cs1 147.488(12) . . ?
W3 Ti2 Cs1 147.488(12) 5 . ?
O24 Ti2 Cs2 76.403(13) . 8_665 ?
O22 Ti2 Cs2 48.14(8) . 8_665 ?
O22 Ti2 Cs2 134.72(7) 5 8_665 ?
O10 Ti2 Cs2 135.04(8) 5 8_665 ?
O10 Ti2 Cs2 51.90(8) . 8_665 ?
O13 Ti2 Cs2 103.659(12) . 8_665 ?
W3 Ti2 Cs2 70.108(7) . 8_665 ?
W3 Ti2 Cs2 130.403(19) 5 8_665 ?
Cs1 Ti2 Cs2 81.735(12) . 8_665 ?
O24 Ti2 Cs2 76.405(13) . 9_465 ?
O22 Ti2 Cs2 134.71(8) . 9_465 ?
O22 Ti2 Cs2 48.14(8) 5 9_465 ?
O10 Ti2 Cs2 51.90(8) 5 9_465 ?
O10 Ti2 Cs2 135.04(8) . 9_465 ?
O13 Ti2 Cs2 103.657(12) . 9_465 ?
W3 Ti2 Cs2 130.401(19) . 9_465 ?
W3 Ti2 Cs2 70.106(7) 5 9_465 ?
Cs1 Ti2 Cs2 81.737(12) . 9_465 ?
Cs2 Ti2 Cs2 152.56(2) 8_665 9_465 ?
O24 Ti3 O24 98.23(17) 2_665 3_565 ?
O24 Ti3 O24 98.23(17) 2_665 . ?
O24 Ti3 O24 98.23(17) 3_565 . ?
O24 Ti3 O25 89.14(16) 2_665 2_665 ?
O24 Ti3 O25 89.14(16) 3_565 2_665 ?
O24 Ti3 O25 168.7(2) . 2_665 ?
O24 Ti3 O25 89.13(16) 2_665 . ?
O24 Ti3 O25 168.7(2) 3_565 . ?
O24 Ti3 O25 89.13(16) . . ?
O25 Ti3 O25 82.4(3) 2_665 . ?
O24 Ti3 O25 168.7(2) 2_665 3_565 ?
O24 Ti3 O25 89.14(16) 3_565 3_565 ?
O24 Ti3 O25 89.13(16) . 3_565 ?
O25 Ti3 O25 82.4(3) 2_665 3_565 ?
O25 Ti3 O25 82.4(3) . 3_565 ?
O24 Ti3 Cs1 60.80(13) 2_665 . ?
O24 Ti3 Cs1 60.81(13) 3_565 . ?
O24 Ti3 Cs1 60.81(13) . . ?
O25 Ti3 Cs1 130.5(2) 2_665 . ?
O25 Ti3 Cs1 130.5(2) . . ?
O25 Ti3 Cs1 130.5(2) 3_565 . ?
O13 Si1 O17 109.99(12) . 5 ?
O13 Si1 O17 109.99(12) . . ?
O17 Si1 O17 109.60(18) 5 . ?
O13 Si1 O4 109.07(19) . . ?
O17 Si1 O4 109.09(11) 5 . ?
O17 Si1 O4 109.09(11) . . ?
W1 O1 Cs2 125.6(2) . . ?
W1 O1 Cs4 103.48(17) . . ?
Cs2 O1 Cs4 130.97(16) . . ?
W1 O2 W5 150.97(17) . 5 ?
W1 O2 Cs3 105.44(10) . 5 ?
W5 O2 Cs3 102.56(10) 5 5 ?
W1 O2 Cs4 84.98(9) . . ?
W5 O2 Cs4 94.49(11) 5 . ?
Cs3 O2 Cs4 106.24(8) 5 . ?
W2 O3 W1 120.95(11) 5 . ?
W2 O3 Cs3 102.56(12) 5 . ?
W1 O3 Cs3 105.08(12) . . ?
Si1 O4 W1 123.8(2) . . ?
Si1 O4 W2 124.52(12) . . ?
W1 O4 W2 91.52(10) . . ?
Si1 O4 W2 124.52(12) . 5 ?
W1 O4 W2 91.52(10) . 5 ?
W2 O4 W2 91.09(12) . 5 ?
W2 O5 Na1 160.6(5) . . ?
W2 O5 Cs3 96.82(9) . 12_465 ?
Na1 O5 Cs3 87.3(3) . 12_465 ?
W2 O6 W3 152.12(17) . 5 ?
W2 O6 Cs3 91.89(11) . 12_465 ?
W3 O6 Cs3 85.31(9) 5 12_465 ?
W2 O7 W4 151.70(18) . 5 ?
W2 O7 Cs3 105.53(9) . 5 ?
W4 O7 Cs3 102.06(11) 5 5 ?
W2 O7 Cs3 92.41(11) . 12_465 ?
W4 O7 Cs3 84.62(9) 5 12_465 ?
Cs3 O7 Cs3 108.63(8) 5 12_465 ?
W2 O8 W2 120.59(19) 5 . ?
W3 O9 Na1 143.0(4) . 10_665 ?
W3 O9 Cs3 101.02(12) . 8_665 ?
Na1 O9 Cs3 108.6(3) 10_665 8_665 ?
W3 O10 Ti2 117.66(15) . . ?
W3 O10 Cs2 111.97(10) . 8_665 ?
Ti2 O10 Cs2 98.69(10) . 8_665 ?
W4 O11 W3 153.75(17) . . ?
W4 O11 Cs3 92.13(7) . 8_665 ?
W3 O11 Cs3 93.17(9) . 8_665 ?
W4 O11 Cs2 102.11(10) . 8_665 ?
W3 O11 Cs2 100.09(9) . 8_665 ?
Cs3 O11 Cs2 110.28(8) 8_665 8_665 ?
W3 O12 W3 119.58(19) . 5 ?
Si1 O13 Ti2 122.23(19) . . ?
Si1 O13 W3 125.03(11) . . ?
Ti2 O13 W3 92.09(11) . . ?
Si1 O13 W3 125.03(10) . 5 ?
Ti2 O13 W3 92.09(11) . 5 ?
W3 O13 W3 90.75(13) . 5 ?
W4 O14 Cs3 101.07(13) . 8_665 ?
W4 O14 Cs4 136.82(13) . 8_665 ?
Cs3 O14 Cs4 115.90(9) 8_665 8_665 ?
W4 O15 Ti1 117.38(15) . . ?
W4 O15 K1 110.41(11) . . ?
Ti1 O15 K1 106.46(15) . . ?
W4 O15 Cs2 111.63(11) . 8_665 ?
Ti1 O15 Cs2 95.61(8) . 8_665 ?
K1 O15 Cs2 114.74(10) . 8_665 ?
W4 O16 W5 119.87(13) . . ?
W4 O16 Cs3 105.71(10) . . ?
W5 O16 Cs3 109.22(12) . . ?
Si1 O17 Ti1 123.56(11) . . ?
Si1 O17 W5 125.59(15) . . ?
Ti1 O17 W5 92.43(10) . . ?
Si1 O17 W4 124.64(13) . . ?
Ti1 O17 W4 89.35(10) . . ?
W5 O17 W4 90.96(8) . . ?
W5 O18 Cs4 100.92(15) . . ?
W5 O19 Ti1 118.11(14) . . ?
W5 O20 W5 154.2(2) 5 . ?
W5 O20 Cs4 90.30(11) 5 . ?
W5 O20 Cs4 90.30(11) . . ?
Ti1 O21 Ti1 152.3(2) 6_565 . ?
Ti1 O21 Cs1 92.03(12) 6_565 . ?
Ti1 O21 Cs1 92.03(12) . . ?
Ti1 O22 Ti2 147.55(17) . . ?
Ti1 O22 Cs2 104.66(11) . 8_665 ?
Ti2 O22 Cs2 105.56(10) . 8_665 ?
Ti1 O22 Cs1 90.74(8) . . ?
Ti2 O22 Cs1 91.52(7) . . ?
Cs2 O22 Cs1 107.05(7) 8_665 . ?
Ti1 O23 Ti1 137.4(2) . 5 ?
Ti1 O23 Cs1 89.14(11) . . ?
Ti1 O23 Cs1 89.14(11) 5 . ?
Ti3 O24 Ti2 178.1(2) . . ?
Ti3 O24 Cs1 90.85(14) . . ?
Ti2 O24 Cs1 91.02(15) . . ?
O23 Cs1 O23 97.95(9) . 2_665 ?
O23 Cs1 O23 97.95(9) . 3_565 ?
O23 Cs1 O23 97.95(9) 2_665 3_565 ?
O23 Cs1 O21 126.98(10) . 3_565 ?
O23 Cs1 O21 53.43(3) 2_665 3_565 ?
O23 Cs1 O21 53.43(3) 3_565 3_565 ?
O23 Cs1 O21 53.43(3) . 2_665 ?
O23 Cs1 O21 53.43(3) 2_665 2_665 ?
O23 Cs1 O21 126.98(10) 3_565 2_665 ?
O21 Cs1 O21 105.04(8) 3_565 2_665 ?
O23 Cs1 O21 53.43(3) . . ?
O23 Cs1 O21 126.98(10) 2_665 . ?
O23 Cs1 O21 53.43(3) 3_565 . ?
O21 Cs1 O21 105.03(8) 3_565 . ?
O21 Cs1 O21 105.03(8) 2_665 . ?
O23 Cs1 O22 49.45(7) . . ?
O23 Cs1 O22 143.86(5) 2_665 . ?
O23 Cs1 O22 101.42(5) 3_565 . ?
O21 Cs1 O22 154.84(5) 3_565 . ?
O21 Cs1 O22 90.74(5) 2_665 . ?
O21 Cs1 O22 51.08(7) . . ?
O23 Cs1 O22 143.86(5) . 4_665 ?
O23 Cs1 O22 49.45(7) 2_665 4_665 ?
O23 Cs1 O22 101.42(5) 3_565 4_665 ?
O21 Cs1 O22 51.08(7) 3_565 4_665 ?
O21 Cs1 O22 90.74(5) 2_665 4_665 ?
O21 Cs1 O22 154.84(5) . 4_665 ?
O22 Cs1 O22 150.10(9) . 4_665 ?
O23 Cs1 O22 101.42(5) . 2_665 ?
O23 Cs1 O22 49.45(7) 2_665 2_665 ?
O23 Cs1 O22 143.86(5) 3_565 2_665 ?
O21 Cs1 O22 90.74(5) 3_565 2_665 ?
O21 Cs1 O22 51.08(7) 2_665 2_665 ?
O21 Cs1 O22 154.84(5) . 2_665 ?
O22 Cs1 O22 114.37(3) . 2_665 ?
O22 Cs1 O22 47.66(10) 4_665 2_665 ?
O23 Cs1 O22 143.86(5) . 3_565 ?
O23 Cs1 O22 101.42(5) 2_665 3_565 ?
O23 Cs1 O22 49.45(7) 3_565 3_565 ?
O21 Cs1 O22 51.08(7) 3_565 3_565 ?
O21 Cs1 O22 154.84(5) 2_665 3_565 ?
O21 Cs1 O22 90.74(5) . 3_565 ?
O22 Cs1 O22 114.37(3) . 3_565 ?
O22 Cs1 O22 68.41(10) 4_665 3_565 ?
O22 Cs1 O22 114.38(4) 2_665 3_565 ?
O23 Cs1 O22 101.42(5) . 6_565 ?
O23 Cs1 O22 143.86(5) 2_665 6_565 ?
O23 Cs1 O22 49.45(7) 3_565 6_565 ?
O21 Cs1 O22 90.74(5) 3_565 6_565 ?
O21 Cs1 O22 154.84(5) 2_665 6_565 ?
O21 Cs1 O22 51.08(7) . 6_565 ?
O22 Cs1 O22 68.41(10) . 6_565 ?
O22 Cs1 O22 114.38(3) 4_665 6_565 ?
O22 Cs1 O22 150.10(9) 2_665 6_565 ?
O22 Cs1 O22 47.66(10) 3_565 6_565 ?
O23 Cs1 O22 49.44(7) . 5 ?
O23 Cs1 O22 101.42(5) 2_665 5 ?
O23 Cs1 O22 143.86(5) 3_565 5 ?
O21 Cs1 O22 154.84(5) 3_565 5 ?
O21 Cs1 O22 51.08(7) 2_665 5 ?
O21 Cs1 O22 90.74(5) . 5 ?
O22 Cs1 O22 47.66(10) . 5 ?
O22 Cs1 O22 114.38(3) 4_665 5 ?
O22 Cs1 O22 68.41(10) 2_665 5 ?
O22 Cs1 O22 150.10(9) 3_565 5 ?
O22 Cs1 O22 114.37(4) 6_565 5 ?
O1 Cs2 O22 124.06(8) . 16_664 ?
O1 Cs2 O22 124.05(8) . 15_564 ?
O22 Cs2 O22 71.45(8) 16_664 15_564 ?
O1 Cs2 O10 116.69(4) . 16_664 ?
O22 Cs2 O10 51.13(7) 16_664 16_664 ?
O22 Cs2 O10 112.56(5) 15_564 16_664 ?
O1 Cs2 O10 116.68(4) . 15_564 ?
O22 Cs2 O10 112.56(5) 16_664 15_564 ?
O22 Cs2 O10 51.13(7) 15_564 15_564 ?
O10 Cs2 O10 119.97(8) 16_664 15_564 ?
O1 Cs2 O15 74.74(9) . 16_664 ?
O22 Cs2 O15 50.98(6) 16_664 16_664 ?
O22 Cs2 O15 87.39(6) 15_564 16_664 ?
O10 Cs2 O15 82.36(7) 16_664 16_664 ?
O10 Cs2 O15 137.14(7) 15_564 16_664 ?
O1 Cs2 O15 74.74(9) . 15_564 ?
O22 Cs2 O15 87.39(6) 16_664 15_564 ?
O22 Cs2 O15 50.98(6) 15_564 15_564 ?
O10 Cs2 O15 137.15(7) 16_664 15_564 ?
O10 Cs2 O15 82.35(7) 15_564 15_564 ?
O15 Cs2 O15 60.02(10) 16_664 15_564 ?
O1 Cs2 O11 76.39(5) . 16_664 ?
O22 Cs2 O11 57.95(5) 16_664 16_664 ?
O22 Cs2 O11 125.81(6) 15_564 16_664 ?
O10 Cs2 O11 46.97(6) 16_664 16_664 ?
O10 Cs2 O11 166.47(6) 15_564 16_664 ?
O15 Cs2 O11 46.64(7) 16_664 16_664 ?
O15 Cs2 O11 105.61(7) 15_564 16_664 ?
O1 Cs2 O11 76.39(4) . 15_564 ?
O22 Cs2 O11 125.81(6) 16_664 15_564 ?
O22 Cs2 O11 57.94(5) 15_564 15_564 ?
O10 Cs2 O11 166.47(6) 16_664 15_564 ?
O10 Cs2 O11 46.96(6) 15_564 15_564 ?
O15 Cs2 O11 105.61(7) 16_664 15_564 ?
O15 Cs2 O11 46.64(7) 15_564 15_564 ?
O11 Cs2 O11 145.68(9) 16_664 15_564 ?
O1 Cs2 Ti1 103.73(9) . 16_664 ?
O22 Cs2 Ti1 25.97(5) 16_664 16_664 ?
O22 Cs2 Ti1 67.40(5) 15_564 16_664 ?
O10 Cs2 Ti1 72.70(5) 16_664 16_664 ?
O10 Cs2 Ti1 117.76(5) 15_564 16_664 ?
O15 Cs2 Ti1 29.29(4) 16_664 16_664 ?
O15 Cs2 Ti1 64.45(4) 15_564 16_664 ?
O11 Cs2 Ti1 58.71(5) 16_664 16_664 ?
O11 Cs2 Ti1 108.84(5) 15_564 16_664 ?
O1 Cs2 Ti1 103.73(9) . 15_564 ?
O22 Cs2 Ti1 67.40(5) 16_664 15_564 ?
O22 Cs2 Ti1 25.97(5) 15_564 15_564 ?
O10 Cs2 Ti1 117.77(5) 16_664 15_564 ?
O10 Cs2 Ti1 72.70(5) 15_564 15_564 ?
O15 Cs2 Ti1 64.45(4) 16_664 15_564 ?
O15 Cs2 Ti1 29.29(4) 15_564 15_564 ?
O11 Cs2 Ti1 108.84(5) 16_664 15_564 ?
O11 Cs2 Ti1 58.71(5) 15_564 15_564 ?
Ti1 Cs2 Ti1 52.301(19) 16_664 15_564 ?
O1 Cs2 Ti2 135.55(3) . 14_664 ?
O22 Cs2 Ti2 26.30(5) 16_664 14_664 ?
O22 Cs2 Ti2 84.07(4) 15_564 14_664 ?
O10 Cs2 Ti2 29.41(4) 16_664 14_664 ?
O10 Cs2 Ti2 107.77(4) 15_564 14_664 ?
O15 Cs2 Ti2 73.00(5) 16_664 14_664 ?
O15 Cs2 Ti2 112.77(4) 15_564 14_664 ?
O11 Cs2 Ti2 59.25(4) 16_664 14_664 ?
O11 Cs2 Ti2 141.87(4) 15_564 14_664 ?
Ti1 Cs2 Ti2 51.957(16) 16_664 14_664 ?
Ti1 Cs2 Ti2 88.994(16) 15_564 14_664 ?
O16 Cs3 O7 49.85(7) . 5 ?
O16 Cs3 O3W 74.1(4) . 18_564 ?
O7 Cs3 O3W 86.6(3) 5 18_564 ?
O16 Cs3 O14 103.11(7) . 15_564 ?
O7 Cs3 O14 126.18(8) 5 15_564 ?
O3W Cs3 O14 135.7(3) 18_564 15_564 ?
O16 Cs3 O3 82.87(7) . . ?
O7 Cs3 O3 48.53(6) 5 . ?
O3W Cs3 O3 133.4(3) 18_564 . ?
O14 Cs3 O3 88.49(8) 15_564 . ?
O16 Cs3 O9 141.95(8) . 15_564 ?
O7 Cs3 O9 92.12(7) 5 15_564 ?
O3W Cs3 O9 109.2(4) 18_564 15_564 ?
O14 Cs3 O9 99.43(7) 15_564 15_564 ?
O3 Cs3 O9 67.41(7) . 15_564 ?
O16 Cs3 O2 49.05(7) . 5 ?
O7 Cs3 O2 57.13(8) 5 5 ?
O3W Cs3 O2 123.1(4) 18_564 5 ?
O14 Cs3 O2 70.27(7) 15_564 5 ?
O3 Cs3 O2 47.87(6) . 5 ?
O9 Cs3 O2 113.87(7) 15_564 5 ?
O16 Cs3 O11 149.62(8) . 15_564 ?
O7 Cs3 O11 128.04(6) 5 15_564 ?
O3W Cs3 O11 134.3(4) 18_564 15_564 ?
O14 Cs3 O11 50.82(6) 15_564 15_564 ?
O3 Cs3 O11 81.32(7) . 15_564 ?
O9 Cs3 O11 50.14(7) 15_564 15_564 ?
O2 Cs3 O11 102.04(6) 5 15_564 ?
O16 Cs3 O5 119.36(8) . 18_564 ?
O7 Cs3 O5 141.71(8) 5 18_564 ?
O3W Cs3 O5 56.8(3) 18_564 18_564 ?
O14 Cs3 O5 90.95(8) 15_564 18_564 ?
O3 Cs3 O5 157.18(7) . 18_564 ?
O9 Cs3 O5 90.22(9) 15_564 18_564 ?
O2 Cs3 O5 151.08(8) 5 18_564 ?
O11 Cs3 O5 80.69(7) 15_564 18_564 ?
O16 Cs3 O7 134.80(8) . 18_564 ?
O7 Cs3 O7 170.92(5) 5 18_564 ?
O3W Cs3 O7 102.1(3) 18_564 18_564 ?
O14 Cs3 O7 48.15(7) 15_564 18_564 ?
O3 Cs3 O7 122.39(6) . 18_564 ?
O9 Cs3 O7 82.66(8) 15_564 18_564 ?
O2 Cs3 O7 118.35(6) 5 18_564 ?
O11 Cs3 O7 43.30(6) 15_564 18_564 ?
O5 Cs3 O7 46.18(6) 18_564 18_564 ?
O16 Cs3 O6 164.79(7) . 18_564 ?
O7 Cs3 O6 136.71(8) 5 18_564 ?
O3W Cs3 O6 91.8(4) 18_564 18_564 ?
O14 Cs3 O6 82.82(7) 15_564 18_564 ?
O3 Cs3 O6 111.52(6) . 18_564 ?
O9 Cs3 O6 47.91(8) 15_564 18_564 ?
O2 Cs3 O6 144.97(5) 5 18_564 ?
O11 Cs3 O6 42.95(6) 15_564 18_564 ?
O5 Cs3 O6 45.89(7) 18_564 18_564 ?
O7 Cs3 O6 41.65(7) 18_564 18_564 ?
O16 Cs3 W4 128.31(6) . 15_564 ?
O7 Cs3 W4 141.84(5) 5 15_564 ?
O3W Cs3 W4 131.4(3) 18_564 15_564 ?
O14 Cs3 W4 25.39(5) 15_564 15_564 ?
O3 Cs3 W4 94.63(6) . 15_564 ?
O9 Cs3 W4 79.14(5) 15_564 15_564 ?
O2 Cs3 W4 92.43(5) 5 15_564 ?
O11 Cs3 W4 29.05(5) 15_564 15_564 ?
O5 Cs3 W4 75.96(6) 18_564 15_564 ?
O7 Cs3 W4 29.79(3) 18_564 15_564 ?
O6 Cs3 W4 57.70(5) 18_564 15_564 ?
O5W Cs4 O1 164.4(8) 1_554 . ?
O5W Cs4 O14 122.61(19) 1_554 16_664 ?
O1 Cs4 O14 61.98(7) . 16_664 ?
O5W Cs4 O14 122.60(19) 1_554 15_564 ?
O1 Cs4 O14 61.98(7) . 15_564 ?
O14 Cs4 O14 110.61(9) 16_664 15_564 ?
O5W Cs4 O9W 20.7(9) 1_554 1_554 ?
O1 Cs4 O9W 174.9(5) . 1_554 ?
O14 Cs4 O9W 116.0(2) 16_664 1_554 ?
O14 Cs4 O9W 116.0(2) 15_564 1_554 ?
O5W Cs4 O10W 38.4(12) 1_554 1_554 ?
O1 Cs4 O10W 157.1(9) . 1_554 ?
O14 Cs4 O10W 107.9(5) 16_664 1_554 ?
O14 Cs4 O10W 107.9(5) 15_564 1_554 ?
O9W Cs4 O10W 17.7(10) 1_554 1_554 ?
O5W Cs4 O3W 71.4(3) 1_554 10_664 ?
O1 Cs4 O3W 109.8(3) . 10_664 ?
O14 Cs4 O3W 157.5(3) 16_664 10_664 ?
O14 Cs4 O3W 51.5(2) 15_564 10_664 ?
O9W Cs4 O3W 70.1(3) 1_554 10_664 ?
O10W Cs4 O3W 71.2(3) 1_554 10_664 ?
O5W Cs4 O3W 71.4(3) 1_554 9_464 ?
O1 Cs4 O3W 109.8(3) . 9_464 ?
O14 Cs4 O3W 51.5(2) 16_664 9_464 ?
O14 Cs4 O3W 157.6(3) 15_564 9_464 ?
O9W Cs4 O3W 70.1(3) 1_554 9_464 ?
O10W Cs4 O3W 71.2(3) 1_554 9_464 ?
O3W Cs4 O3W 140.3(5) 10_664 9_464 ?
O5W Cs4 K1 102.5(8) 1_554 15_564 ?
O1 Cs4 K1 93.05(12) . 15_564 ?
O14 Cs4 K1 72.79(7) 16_664 15_564 ?
O14 Cs4 K1 72.78(7) 15_564 15_564 ?
O9W Cs4 K1 81.8(5) 1_554 15_564 ?
O10W Cs4 K1 64.1(9) 1_554 15_564 ?
O3W Cs4 K1 87.5(3) 10_664 15_564 ?
O3W Cs4 K1 87.5(3) 9_464 15_564 ?
O5W Cs4 O8W 23.8(9) 1_554 . ?
O1 Cs4 O8W 140.6(5) . . ?
O14 Cs4 O8W 124.54(6) 16_664 . ?
O14 Cs4 O8W 124.54(6) 15_564 . ?
O9W Cs4 O8W 44.6(7) 1_554 . ?
O10W Cs4 O8W 62.3(10) 1_554 . ?
O3W Cs4 O8W 75.8(3) 10_664 . ?
O3W Cs4 O8W 75.8(3) 9_464 . ?
K1 Cs4 O8W 126.4(5) 15_564 . ?
O5W Cs4 O18 75.4(6) 1_554 5 ?
O1 Cs4 O18 93.45(8) . 5 ?
O14 Cs4 O18 71.98(6) 16_664 5 ?
O14 Cs4 O18 145.94(9) 15_564 5 ?
O9W Cs4 O18 90.3(4) 1_554 5 ?
O10W Cs4 O18 102.9(7) 1_554 5 ?
O3W Cs4 O18 130.5(3) 10_664 5 ?
O3W Cs4 O18 49.3(3) 9_464 5 ?
K1 Cs4 O18 135.66(5) 15_564 5 ?
O8W Cs4 O18 59.8(3) . 5 ?
O5W Cs4 O18 75.4(6) 1_554 . ?
O1 Cs4 O18 93.45(8) . . ?
O14 Cs4 O18 145.94(9) 16_664 . ?
O14 Cs4 O18 71.97(6) 15_564 . ?
O9W Cs4 O18 90.3(4) 1_554 . ?
O10W Cs4 O18 102.9(7) 1_554 . ?
O3W Cs4 O18 49.3(3) 10_664 . ?
O3W Cs4 O18 130.5(3) 9_464 . ?
K1 Cs4 O18 135.66(5) 15_564 . ?
O8W Cs4 O18 59.8(3) . . ?
O18 Cs4 O18 87.57(9) 5 . ?
O10W K1 O15 134.3(6) 8_664 6_565 ?
O10W K1 O15 134.3(6) 8_664 . ?
O15 K1 O15 63.72(13) 6_565 . ?
O10W K1 O1W 121.4(8) 8_664 . ?
O15 K1 O1W 92.8(2) 6_565 . ?
O15 K1 O1W 92.8(2) . . ?
O10W K1 Cs4 59.7(8) 8_664 8_665 ?
O15 K1 Cs4 86.23(12) 6_565 8_665 ?
O15 K1 Cs4 86.23(12) . 8_665 ?
O1W K1 Cs4 178.9(3) . 8_665 ?
O10W K1 Ti1 154.37(14) 8_664 6_565 ?
O15 K1 Ti1 27.13(6) 6_565 6_565 ?
O15 K1 Ti1 63.90(10) . 6_565 ?
O1W K1 Ti1 66.0(2) . 6_565 ?
Cs4 K1 Ti1 113.03(12) 8_665 6_565 ?
O10W K1 Ti1 154.36(14) 8_664 . ?
O15 K1 Ti1 63.90(9) 6_565 . ?
O15 K1 Ti1 27.13(6) . . ?
O1W K1 Ti1 66.0(2) . . ?
Cs4 K1 Ti1 113.03(12) 8_665 . ?
Ti1 K1 Ti1 50.47(6) 6_565 . ?
O10W K1 Cs2 133.9(8) 8_664 8_665 ?
O15 K1 Cs2 33.62(7) 6_565 8_665 ?
O15 K1 Cs2 33.62(7) . 8_665 ?
O1W K1 Cs2 104.7(3) . 8_665 ?
Cs4 K1 Cs2 74.21(9) 8_665 8_665 ?
Ti1 K1 Cs2 47.28(5) 6_565 8_665 ?
Ti1 K1 Cs2 47.28(5) . 8_665 ?
Na2 Na1 O3W 78.7(9) 16_665 . ?
Na2 Na1 O5 90.8(8) 16_665 . ?
O3W Na1 O5 87.9(8) . . ?
Na2 Na1 O9 112.3(8) 16_665 16_664 ?
O3W Na1 O9 167.2(7) . 16_664 ?
O5 Na1 O9 85.4(6) . 16_664 ?
Na2 Na1 O9W 73.3(9) 16_665 14_664 ?
O3W Na1 O9W 96.7(9) . 14_664 ?
O5 Na1 O9W 162.1(8) . 14_664 ?
O9 Na1 O9W 93.0(8) 16_664 14_664 ?
Na2 Na1 Cs3 117.0(8) 16_665 12_465 ?
O3W Na1 Cs3 50.2(4) . 12_465 ?
O5 Na1 Cs3 58.2(3) . 12_465 ?
O9 Na1 Cs3 117.1(5) 16_664 12_465 ?
O9W Na1 Cs3 136.4(8) 14_664 12_465 ?
Na2 Na1 Cs4 73.5(8) 16_665 14_665 ?
O3W Na1 Cs4 49.9(6) . 14_665 ?
O5 Na1 Cs4 136.7(6) . 14_665 ?
O9 Na1 Cs4 137.9(6) 16_664 14_665 ?
O9W Na1 Cs4 47.1(6) 14_664 14_665 ?
Cs3 Na1 Cs4 92.9(3) 12_465 14_665 ?
Na2 Na1 Cs3 139.7(8) 16_665 5 ?
O3W Na1 Cs3 126.7(6) . 5 ?
O5 Na1 Cs3 63.2(4) . 5 ?
O9 Na1 Cs3 40.6(3) 16_664 5 ?
O9W Na1 Cs3 124.8(8) 14_664 5 ?
Cs3 Na1 Cs3 76.6(2) 12_465 5 ?
Cs4 Na1 Cs3 146.4(3) 14_665 5 ?
Na1 Na2 O8W 121.0(11) 10_664 . ?
Na1 Na2 O5W 85.7(10) 10_664 1_554 ?
O8W Na2 O5W 36.7(8) . 1_554 ?
Na1 Na2 O3W 56.3(7) 10_664 10_664 ?
O8W Na2 O3W 106.2(9) . 10_664 ?
O5W Na2 O3W 78.4(8) 1_554 10_664 ?
Na1 Na2 Cs4 80.7(7) 10_664 . ?
O8W Na2 Cs4 54.5(7) . . ?
O5W Na2 Cs4 27.9(6) 1_554 . ?
O3W Na2 Cs4 52.9(5) 10_664 . ?
Na1 O3W Na2 45.0(6) . 16_665 ?
Na1 O3W Cs3 96.7(6) . 12_465 ?
Na2 O3W Cs3 128.5(7) 16_665 12_465 ?
Na1 O3W Cs4 99.3(7) . 14_665 ?
Na2 O3W Cs4 88.1(5) 16_665 14_665 ?
Cs3 O3W Cs4 138.8(6) 12_465 14_665 ?
O9W O5W O8W 113(3) . 1_556 ?
O9W O5W Cs4 124(2) . 1_556 ?
O8W O5W Cs4 123.5(19) 1_556 1_556 ?
O9W O5W Na2 83.0(11) . 5_556 ?
O8W O5W Na2 67.1(8) 1_556 5_556 ?
Cs4 O5W Na2 117.3(7) 1_556 5_556 ?
O9W O5W Na2 83.0(11) . 1_556 ?
O8W O5W Na2 67.1(8) 1_556 1_556 ?
Cs4 O5W Na2 117.3(7) 1_556 1_556 ?
Na2 O5W Na2 121.7(12) 5_556 1_556 ?
O6W O6W O6W 60.00(2) 2_665 3_565 ?
O5W O8W Na2 76.2(8) 1_554 5 ?
O5W O8W Na2 76.2(8) 1_554 . ?
Na2 O8W Na2 134.1(14) 5 . ?
O5W O8W Cs4 32.6(12) 1_554 . ?
Na2 O8W Cs4 88.1(7) 5 . ?
Na2 O8W Cs4 88.1(7) . . ?
O5W O9W Na1 95.3(7) . 10_665 ?
O5W O9W Na1 95.3(7) . 9_465 ?
Na1 O9W Na1 168.9(14) 10_665 9_465 ?
O5W O9W Cs4 35.3(16) . 1_556 ?
Na1 O9W Cs4 93.3(7) 10_665 1_556 ?
Na1 O9W Cs4 93.3(7) 9_465 1_556 ?
K1 O10W Cs4 56.2(8) 15_565 1_556 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O1 1.720(5) . ?
W1 O2 1.860(2) 5 ?
W1 O2 1.860(2) . ?
W1 O3 1.935(3) . ?
W1 O3 1.935(3) 5 ?
W1 O4 2.345(4) . ?
W1 Cs4 3.8784(17) . ?
W1 Cs3 4.2019(4) 5 ?
W1 Cs3 4.2020(4) . ?
W1 Cs2 4.2843(5) . ?
W2 O5 1.736(3) . ?
W2 O7 1.868(2) . ?
W2 O6 1.877(3) . ?
W2 O3 1.935(3) 5 ?
W2 O8 1.9354(19) . ?
W2 O4 2.355(2) . ?
W2 Cs3 4.1363(4) 12_465 ?
W2 Cs3 4.1374(5) 5 ?
W3 O9 1.723(3) . ?
W3 O10 1.836(2) . ?
W3 O11 1.918(3) . ?
W3 O12 1.9430(19) . ?
W3 O6 1.963(3) 5 ?
W3 O13 2.359(3) . ?
W3 Ti2 3.3005(7) . ?
W3 Cs3 3.9788(3) 8_665 ?
W3 Cs2 4.2776(3) 8_665 ?
W4 O14 1.726(3) . ?
W4 O15 1.839(2) . ?
W4 O11 1.919(3) . ?
W4 O16 1.935(3) . ?
W4 O7 1.971(2) 5 ?
W4 O17 2.375(2) . ?
W4 Ti1 3.2551(5) . ?
W4 Cs3 3.9497(5) 8_665 ?
W4 Cs3 4.1162(4) . ?
W4 Cs2 4.3323(4) 8_665 ?
W5 O18 1.719(3) . ?
W5 O19 1.849(2) . ?
W5 O20 1.9162(9) . ?
W5 O16 1.947(3) . ?
W5 O2 1.988(2) 5 ?
W5 O17 2.338(3) . ?
W5 Ti1 3.3147(6) . ?
W5 Cs3 4.2106(3) . ?
W5 Cs4 4.2196(15) . ?
Ti1 O22 1.814(3) . ?
Ti1 O21 1.8192(11) . ?
Ti1 O15 1.970(2) . ?
Ti1 O23 2.0115(16) . ?
Ti1 O19 2.015(3) . ?
Ti1 O17 2.253(2) . ?
Ti1 Cs1 3.7561(5) . ?
Ti1 Cs2 4.0078(8) 8_665 ?
Ti1 K1 4.143(5) . ?
Ti2 O24 1.822(4) . ?
Ti2 O22 1.870(3) . ?
Ti2 O22 1.870(3) 5 ?
Ti2 O10 2.020(2) 5 ?
Ti2 O10 2.020(2) . ?
Ti2 O13 2.224(3) . ?
Ti2 W3 3.3007(7) 5 ?
Ti2 Cs1 3.8062(9) . ?
Ti2 Cs2 4.0667(4) 8_665 ?
Ti2 Cs2 4.0667(4) 9_465 ?
Ti3 O24 1.800(4) 2_665 ?
Ti3 O24 1.800(4) 3_565 ?
Ti3 O24 1.800(4) . ?
Ti3 O25 2.161(7) 2_665 ?
Ti3 O25 2.161(7) . ?
Ti3 O25 2.162(7) 3_565 ?
Ti3 Cs1 3.7908(17) . ?
Si1 O13 1.624(4) . ?
Si1 O17 1.627(3) 5 ?
Si1 O17 1.627(3) . ?
Si1 O4 1.635(3) . ?
O1 Cs2 3.050(4) . ?
O1 Cs4 3.098(5) . ?
O2 W5 1.987(2) 5 ?
O2 Cs3 3.305(3) 5 ?
O2 Cs4 3.570(3) . ?
O3 W2 1.935(3) 5 ?
O3 Cs3 3.260(3) . ?
O4 W2 2.355(2) 5 ?
O5 Na1 2.369(18) . ?
O5 Cs3 3.554(3) 12_465 ?
O6 W3 1.963(3) 5 ?
O6 Cs3 3.625(3) 12_465 ?
O7 W4 1.971(2) 5 ?
O7 Cs3 3.225(3) 5 ?
O7 Cs3 3.613(3) 12_465 ?
O8 W2 1.9354(19) 5 ?
O9 Na1 2.575(19) 10_665 ?
O9 Cs3 3.272(3) 8_665 ?
O10 Cs2 3.237(3) 8_665 ?
O11 Cs3 3.381(2) 8_665 ?
O11 Cs2 3.502(3) 8_665 ?
O12 W3 1.9430(19) 5 ?
O13 W3 2.359(3) 5 ?
O14 Cs3 3.237(3) 8_665 ?
O14 Cs4 3.254(3) 8_665 ?
O15 K1 3.129(5) . ?
O15 Cs2 3.303(3) 8_665 ?
O16 Cs3 3.147(2) . ?
O18 Cs4 3.541(4) . ?
O20 W5 1.9161(9) 5 ?
O20 Cs4 3.749(4) . ?
O21 Ti1 1.8191(11) 6_565 ?
O21 Cs1 3.222(4) . ?
O22 Cs2 3.144(3) 8_665 ?
O22 Cs1 3.2659(19) . ?
O23 Ti1 2.0115(15) 5 ?
O23 Cs1 3.202(4) . ?
O24 Cs1 3.310(4) . ?
Cs1 O23 3.202(4) 2_665 ?
Cs1 O23 3.203(4) 3_565 ?
Cs1 O21 3.222(4) 3_565 ?
Cs1 O21 3.222(4) 2_665 ?
Cs1 O22 3.2659(19) 4_665 ?
Cs1 O22 3.2660(19) 2_665 ?
Cs1 O22 3.2659(19) 3_565 ?
Cs1 O22 3.2660(19) 6_565 ?
Cs1 O22 3.2660(19) 5 ?
Cs2 O22 3.144(3) 16_664 ?
Cs2 O22 3.144(3) 15_564 ?
Cs2 O10 3.237(3) 16_664 ?
Cs2 O10 3.238(3) 15_564 ?
Cs2 O15 3.303(3) 16_664 ?
Cs2 O15 3.303(3) 15_564 ?
Cs2 O11 3.502(3) 16_664 ?
Cs2 O11 3.502(3) 15_564 ?
Cs2 Ti1 4.0077(8) 16_664 ?
Cs2 Ti1 4.0078(8) 15_564 ?
Cs2 Ti2 4.0667(4) 14_664 ?
Cs3 O7 3.225(3) 5 ?
Cs3 O3W 3.233(13) 18_564 ?
Cs3 O14 3.237(3) 15_564 ?
Cs3 O9 3.272(3) 15_564 ?
Cs3 O2 3.305(3) 5 ?
Cs3 O11 3.381(2) 15_564 ?
Cs3 O5 3.554(3) 18_564 ?
Cs3 O7 3.613(3) 18_564 ?
Cs3 O6 3.625(3) 18_564 ?
Cs3 W4 3.9495(5) 15_564 ?
Cs4 O5W 2.26(3) 1_554 ?
Cs4 O14 3.254(3) 16_664 ?
Cs4 O14 3.254(3) 15_564 ?
Cs4 O9W 3.25(3) 1_554 ?
Cs4 O10W 3.64(5) 1_554 ?
Cs4 O3W 3.428(18) 10_664 ?
Cs4 O3W 3.429(18) 9_464 ?
Cs4 K1 3.502(6) 15_564 ?
Cs4 O8W 3.50(3) . ?
Cs4 O18 3.541(4) 5 ?
K1 O10W 3.79(6) 8_664 ?
K1 O15 3.129(5) 6_565 ?
K1 O1W 3.268(16) . ?
K1 Cs4 3.502(6) 8_665 ?
K1 Ti1 4.143(5) 6_565 ?
K1 Cs2 5.418(5) 8_665 ?
Na1 Na2 1.95(2) 16_665 ?
Na1 O3W 2.30(2) . ?
Na1 O9 2.575(19) 16_664 ?
Na1 O9W 2.822(17) 14_664 ?
Na1 Cs3 4.177(14) 12_465 ?
Na1 Cs4 4.424(18) 14_665 ?
Na1 Cs3 4.765(18) 5 ?
Na2 Na1 1.95(2) 10_664 ?
Na2 O8W 2.615(19) . ?
Na2 O5W 2.76(2) 1_554 ?
Na2 O3W 2.70(2) 10_664 ?
O3W Na2 2.70(2) 16_665 ?
O3W Cs3 3.232(13) 12_465 ?
O3W Cs4 3.428(18) 14_665 ?
O5W O9W 1.39(4) . ?
O5W O8W 1.70(4) 1_556 ?
O5W Cs4 2.26(3) 1_556 ?
O5W Na2 2.76(2) 5_556 ?
O5W Na2 2.76(2) 1_556 ?
O6W O6W 0.67(8) 2_665 ?
O6W O6W 0.67(8) 3_565 ?
O8W O5W 1.70(4) 1_554 ?
O8W Na2 2.615(19) 5 ?
O9W Na1 2.822(17) 10_665 ?
O9W Na1 2.822(17) 9_465 ?
O9W Cs4 3.25(3) 1_556 ?
O10W K1 3.79(6) 15_565 ?
O10W Cs4 3.64(5) 1_556 ?
